- Nano Express
- Open Access
Effect of Different CH3NH3PbI3 Morphologies on Photovoltaic Properties of Perovskite Solar Cells
Nanoscale Research Letters volume 13, Article number: 140 (2018)
In this study, the perovskite layers were prepared by two-step wet process with different CH3NH3I (MAI) concentrations. The cell structure was glass/FTO/TiO2-mesoporous/CH3NH3PbI3 (MAPbI3)/spiro-OMeTAD/Ag. The MAPbI3 perovskite films were prepared using high and low MAI concentrations in a two-step process. The perovskite films were optimized at different spin coating speed and different annealing temperatures to enhance the power conversion efficiency (PCE) of perovskite solar cells. The PCE of the resulting device based on the different perovskite morphologies was discussed. The PCE of the best cell was up to 17.42%, open circuit voltage of 0.97 V, short current density of 24.06 mA/cm2, and fill factor of 0.747.
Organic perovskite films have drawn much attention for better power conversion efficiency in thin film-type solar cells [1,2,3]. Many growth methods have been developed to prepare perovskite films. Among them, a two-step method is widely used due to its high film quality and reliability of the resulting films [4, 5]. The perovskite is a versatile material prepared from abundant and low-cost compounds, also having unique optical and long excitonic properties, as well as good electrical conductivity. The power conversion efficiency (PCE) of perovskite solar cells has been improved from 3.8 to 22.1% in recent years.
There are two methods for preparing perovskite films: one-step and two-step methods for CH3NH3PbI3 films; the one-step method is that the PbI2 and CH3NH3I (MAI) are mixed in a solvent to form CH3NH3PbI3 films, such as vacuum flash-assisted solution processes,  solvent engineering,  humidity control, [7, 8] and mixed precursors . Although the one-step method is the most widely used method to prepare the perovskite solar cells, it needs to dissolve both the organic and the inorganic precursors, which reduced the control of the film property including thickness, uniformity, and morphology. The two-step method is that the PbI2 films were first prepared and subsequently reacted with MAI to form CH3NH3PbI3 films. In 2013, Bi et al.  first showed the PCE of 9.5% by using two-step method. They prepare PbI2 films on mesoporous TiO2 films the by spin coating a PbI2 solution in dimethylformamide (DMF). After drying, the films were dipped in a solution of MAI in 2-propanol to form high-quality CH3NH3PbI3 films for the perovskite solar cells. In the same year, Burschka et al.  showed the certification for the perovskite solar cells prepared by the two-step method and confirmed a power conversion efficiency of 14.14% measured under standard AM1.5G reporting conditions. After that, many studies using the two-step method to improve the PCE of the perovskite solar cells were reported [12,13,14,15,16,17,18]. Moreover, long-term stability is important for the future application of perovskite devices. Several nanostructures, like carbon layer  and graphene oxide-modified PEDOT:PSS , have been used to suppress degradation in the device and improve their performance. However, few studies discuss the effect of different surface morphology on photovoltaic properties of perovskite solar cells.
In this study, we controlled the grain size and morphology of CH3NH3PbI3 by different MAI concentration, annealing, and two-step. Moreover, it was found that the surface morphology of CH3NH3PbI3 films using low MAI concentrations showed large perovskite grains, but the morphology of CH3NH3PbI3 films using high MAI concentrations showed dense and smooth grains. Photovoltaic conversion efficiency of the resulting cells based on the different perovskite morphologies was analyzed using XRD spectra, SEM, UV-vis absorption spectroscopy, and photoluminescence (PL) spectra. As a result, the power conversion efficiency of the best cell was up to 17.42%.
In this study, fluorine-doped tin oxide (FTO) glass as substrate was cut into small pieces with a size of 1.5 × 1.5 cm2. The FTO glass substrates were thoroughly cleaned with acetone, ethanol, and deionized (DI) water in an ultrasonic oscillator for 5 min, respectively, and dried with nitrogen. A 50-nm compact TiO2 blocking layer was first deposited onto the surface of the precleaned FTO substrate by spray pyrolysis method at a temperature of 500 °C, using a solution of 0.2 M Ti-isopropoxide and 2 M acetylacetone in isopropanol. The mesoporous layer TiO2 was deposited by spin coating a diluted paste (Dyesol 18NR-T), followed by heating to 450 °C. Next, the two-step method was employed to deposit a perovskite layer. PbI2 (Alfa Aesar, 99.9985% purity) was deposited via spin coating from a solution 1 mol/L PbI2 in dimethylformamide (DMF) that was heated to 70 °C, with a spin coating speed of 7000 rpm. MAPbI3 was formed by dipping the slide into a 10-mg/mL MAII in isopropanol (IPA) solution with different concentrations for 30 s. After removing the excess IPA, the perovskite films were then placed on a hot plate set at 100 °C for 20 min. The composition of hole transport material was 0.170 M 2,2′,7,7′-tetrakis(N,N-di-p-methoxyphenyl-amine)-9,99-spirobifluorene (spiro-OMeTAD, Lumtec), with the addition of 60 mM bis(trifluoromethane)sulfonimide lithium salt (LiTFSI, 99.95%, Aldrich) and 200 mM 4-tert-butylpyridine (TBP, 99%, Aldrich). The CH3NH3PbI3/TiO2 films were coated with a spiro-OMeTAD solution using the spin coating method at 4000 rpm. For the electrical contact, a 100-nm Ag film was deposited onto the solar cell by thermal evaporation. The resultant device was composed of silver/spiro-OMeTAD/MAPbI3/TiO2 mesoporous layer/TiO2 compact layer/FTO/glass. Figure 1 schematically depicts the complete structure. The current density-voltage (J-V) curves of solar cells were obtained using a source measurement unit (Keithly 2400). The photoluminescence spectra of the CN3NH3PbI3/glass samples were measured using a microscope-based spectrometer. The active area of the devices is 2 × 5 mm2 by a shadow mask. The X-ray diffraction patterns of the CN3NH3PbI3/glass samples were recorded using a theta-2theta mode.
Results and Discussion
Figure 2 shows the top-view (left column) and cross-sectional (right column) SEM images of the MAPbI3 perovskite films prepared by low-concentration MAI (10 mg/mL) and underwent annealing treatment at different temperatures. It was found that there is a large amount of perovskite particles on the surface and have a tetragonal morphology, as shown in Fig. 2a. The particles size and surface morphology of the perovskite films prepared by low-concentration MAI are similar for all samples.
Figure 3 shows the top-view (left column) and cross-sectional (right column) SEM images of the MAPbI3 perovskite films prepared by high-concentration MAI (40 mg/mL) and underwent annealing treatment at different temperatures. Perovskite prepared by high-concentration MAI shows tetragonal crystals, the average MAPbI3 domain size from about 200 nm to about 600 nm, as shown in Fig. 3. The morphology is different to that of the perovskite prepared by low-concentration MAI. It was found that there are some PbI2 grains on the surface of the MAPbI3 perovskite film with 60 °C annealing. Those are residues caused by the incomplete reaction. The domain size and surface morphology of the perovskite films prepared by high-concentration MAI are similar for all samples.
Figure 4 shows the XRD patterns of the MAPbI3 films prepared by (a) low- and (b) high-concentration MAI with different annealing temperatures. As shown in Fig. 4a, two main diffraction peaks are observed at 12.6° and 14.4°, corresponding to PbI2 (001) and MAPbI3 (110) phases, respectively. The intensity of the PbI2 (001) peak is higher than that of the MAPbI3 (110) peak when the annealing temperature of the MAPbI3 film increases up to 120 °C. The MAPbI3 film is decomposed into a bi-phase film of the MAI and PbI2, leading to poor efficiency of the perovskite solar cells. Similarly, as shown in Fig. 4b, as the annealing temperature is 60 °C, two main diffraction peaks are observed at 12.8° and 14.3°, corresponding to PbI2 (001) and MAPbI3 (110) phases, respectively. However, the single peak corresponding to the MAPbI3 (110) phase is observed when the annealing temperature of the MAPbI3 film increases up to over 80 °C. The MAI and PbI2 are formed into the MAPbI3 film, completely.
The intensity of photoluminescence (PL) spectrum is related to the lifetime of an exciton in the perovskite film and in the interface between TiO2 and perovskite films. The lifetime of the exciton is longer, and the intensity of PL spectrum is stronger; the decomposition rate of an exciton in the interface between TiO2 and perovskite films is faster, and the intensity of PL spectrum is weaker. Figure 5 plots PL spectra of the MAPbI3 prepared by low- and high-concentration MAI with various spin coating speeds and annealing temperatures. As shown in Fig. 5a, b, the optimum spin coating speed and annealing temperature for the MAPbI3 prepared by low-concentration MAI are 2000 rpm and 100 °C, respectively. On the other hand, as shown in Fig. 5c, d, the optimum spin coating speed and annealing temperature for the MAPbI3 prepared by high-concentration MAI are 4000 rpm and 120 °C, respectively.
Figure 6 shows the SEM images of the MAPbI3 perovskite films with low- and high-concentration MAI solution under optimum conditions, respectively. The surface morphology of the MAPbI3 perovskite films with low-concentration MAI is rougher than that of the MAPbI3 perovskite films with high-concentration MAI. The grain of the latter is compact and smooth. Also, the coverage rate of the surface of the latter is better than that of the former.
Figure 7a shows the PL spectra of the MAPbI3 films with different MAI concentrations. The peak position of PL spectrum increases from 768 to 773 nm when the MAI concentration increases from 10 to 40 mg/mL. The redshift might be associated with the reaction of PbI2 and MAI . As the PbI2 film is reacted with the MAI solution and formed the MAPbI3 perovskite film, the band gap is shifted toward 1.55 eV. Also, the intensity of PL spectrum of the MAPbI3 perovskite film using high MAI concentration is decay. To explore the original cause, time-resolved photoluminescence (TRPL) was employed to study the lifetime of the excitons. Therefore, the excitons can be quickly extracted to the FTO substrate, for the MAPbI3 perovskite film using high MAI concentration. According to the TRPL spectra shown in Fig. 7b, the lifetime of the MAI perovskite films prepared by low and high concentration is 25 and 14 ns, respectively. It can clearly be seen that the exciton lifetime of the MAI perovskite films prepared by high MAI concentration is relatively short, which can be used to explain why the decomposition rate of the excitons is faster. The interface between of TiO2 and perovskite prepared by high MAI concentration is smooth, such that the excitons are separated and extracted quickly to the FTO substrate, as shown in Fig. 7b. In addition, it is possible to improve the film quality, resulting in an increase in the speed of the electrons decomposition.
Figure 8a, b plots the J-V curves of the perovskite solar cells prepared by low- and high-concentration MAI with different annealing temperatures, respectively. To compare the short-circuit current density Jsc, the perovskite solar cells prepared by high-concentration MAI are higher around 2 mA/cm2 than that of the cells prepared by low-concentration MAI. This may be contributed by better quality of the perovskite films prepared by high-concentration MAI, such that it has a higher absorbance, resulting in a higher photocurrent. Besides, the charge transfer resistance in the perovskite films prepared by high-concentration MAI is small due to the smooth morphology. The films with the smooth morphology can not only increase the contact area between perovskite film and spiro-MeTAD film but also enhance the photoelectric conversion efficiency of solar cells [22, 23]. On the other hand, the cells prepared by low-concentration MAI show high Voc. It may be caused by PbI2 residues in the perovskite thin film [22, 23]. To check the reproducibility of performance, power conversion efficiency (PCE) is compared using histograms obtained from 50 perovskite devices prepared by low- and high-concentration MAI, as shown in Fig. 8c. As can be seen from the results, the devices performed extremely well. The average PCE of the perovskite solar cells prepared by low- and high-concentration MAI is 13 and 13.7% with a standard deviation of 1.293 and 1.275%, respectively. As shown in Fig. 8c, more than 75% of the cells show PCE above 13% under one sun conditions, for the perovskite solar cells prepared by high-concentration MAI. That indicates good reproducibility. The optimum results show the power conversion efficiency of 17.42%, open-circuit voltage of 0.97 V, current density of 24.06 mA/cm2, and fill factor of 0.747.
In this study, the perovskite films prepared by high-concentration MAI were used to form solar cells. The effects of different morphologies of the films on the solar cells were investigated. The J-V characteristic curve of perovskite solar cells was used to improve the photoelectric conversion efficiency. The results show that the power conversion efficiency was up to 17.42%, open circuit voltage of 0.97 V, current density of 24.06 mA/cm2, and fill factor of 74.66% was the best characteristic.
Fluorine-doped tin oxide
- MAPbI3 :
Power conversion efficiency
Scanning electron microscope
Dubey A, Adhikari N, Mabrouk S, Wu F, Chen K, Yang S, Qiao Q (2018) A strategic review on processing routes towards highly efficient perovskite solar cells. J Mater Chem A 6(6):2406–2431
Dubey A, Adhikari N, Venkatesan S, Gu S, Khatiwada D, Wang Q, Mohammad L, Kumar M, Qiao Q (2016) Solution processed pristine PDPP3T polymer as hole transport layer for efficient perovskite solar cells with slower degradation. Sol Energy Mater Sol Cells 145:193–199
Tseng Z-L, Chiang C-H, Wu CG (2015) Surface engineering of ZnO thin film for high efficiency planar perovskite solar cells. Sci Rep 5:13211
Jeon N-J, Noh J-H, Kim Y-C, Yang W-S, Ryu S, Seok SI (2014) Solvent engineering for high-performance inorganic–organic hybrid perovskite solar cells. Nat Mater 13:897–903
Li X, Bi D, Yi C, Décoppet J-D, Luo J, Zakeeruddin S-M, Hagfeldt A, Grätzel M (2016) A vacuum flash–assisted solution process for high-efficiency large-area perovskite solar cells. Science 09:58–62
Wu W-Q, Chen DH, McMaster WA, Cheng Y-B, Caruso RA (2017) Solvent-mediated intragranular-coarsening of CH3NH3PbI3 thin films toward high-performance perovskite photovoltaics. ACS Appl Mater Interfaces 9:31959
Dubey A, Kantack N, Adhikari N, Reza KM, Venkatesan S, Kumar M, Khatiwada D, Darling S, Qiao Q (2016) Room temperature, air crystallized perovskite film for high performance solar cells. J Mater Chem A 4(26):10231–10240
Adhikari N, Dubey A, Gaml EA, Vaagensmith B, Reza KM, Mabrouk SAA, Gu SP, Zai JT, Qian XF, Qiao QQ (2016) Crystallization of a perovskite film for higher performance solar cells by controlling water concentration in methyl ammonium iodide precursor solution. Nano 8(5):2693–2703
Khatiwada D, Venkatesan S, Adhikari N, Dubey A, Mitul A, Mohammad L, Iefanova A, Darling SB, Qiao QQ (2015) Efficient perovskite solar cells by temperature control in single and mixed halide precursor solutions and films. J Phys Chem C 119(46):25747–25753
Bi D, Moon S-J, Häggman L, Boschloo G, Yang L, Johansson Erik MJ, Nazeeruddin M-K, Grätzel M, Hagfeldt A (2013) Using a two-step deposition technique to prepare perovskite (CH3NH3PbI3) for thin film solar cells based on ZrO2 and TiO2 mesostructure. RSC Adv 3:18762
Burschka J, Pellet N, Moon S-J, Robin H-B, Gao P, Nazeeruddin M-K, Grätzel M (2013) Sequential deposition as a route to high-performance perovskite-sensitized solar cells. Nature 499:316–319
Mo J, Zhang C, Chang J, Yang H, Xi H, Chen D, Lin Z, Lu G, Zhang J, Haoa Y (2017) Enhanced efficiency of planar perovskite solar cells via a two-step deposition using DMF as an additive to optimize the crystal growth behavior. J Mater Chem A 5:13032
Wang S, Yu W, Zhang L, Yang Y (2017) Crystallization process of PbI2 solution in two-step deposition of CH3NH3PbI3 for high-performance perovskite solar cells. Sol Energy Mater Sol Cells 161:444–448
Abzieher T, Mathies F, Hetterich M, Welle A, Gerthsen D, Lemmer U, Paetzold UW, Powalla M (2017) Additive-assisted crystallization dynamics in two-step fabrication of perovskite solar cells. Phys Status Solidi A 214:1700509
Bahtiar A, Rahmanita S, Inayatie YD (2017) Pin-hole free perovskite film for solar cells application prepared by controlled two-step spin-coating method. IOP Conf Ser: Mater Sci Eng 196:012037
Huang J, Wang M, Ding L, Deng J, Yao X (2015) Efficiency enhancement of the MAPbI3−xClx-based perovskite solar cell by a two-step annealing procedure. Semicond Sci Technol 31(2):025009
Tress W, Marinova N, Moehl T, Zakeeruddin SM, Nazeeruddina MK, Grätzela M (2015) Understanding the rate-dependent J–V hysteresis, slow time component, and aging in CH3NH3PbI3 perovskite solar cells: the role of a compensated electric field. Energy Environ Sci 8(3):995–1004
Wei J, Zhao Y, Li H, Li G, Pan J, Xu D, Zhao Q, Yu D (2014) Hysteresis analysis based on the ferroelectric effect in hybrid perovskite solar cells. J Phys Chem Lett 5(21):3937–3945
Bi E, Chen H, Xie F, Wu Y, Chen W, Su Y, IsIam A, Grätzel M, Yang X, Han L (2017) Diffusion engineering of ions and charge carriers for stable efficient perovskite solar cells. Nat Commun 8:15330
Luo H, Lin X, Hou X, Pan L, Huang S, Chen X (2017) Efficient and air-stable planar perovskite solar cells formed on graphene-oxide-modified PEDOT: PSS hole transport layer. Nano-Micro Lett 9(4):39
Li B, Jiu T, Kuang C, Ma S, Chea Q, Li X, Fang J (2016) Chlorobenzene vapor assistant annealing method for fabricating high quality perovskite films. Org Electron 34:97–103
Tripathi N, Yanagida M, Shirai Y, Masuda T, Hanb L, Miyanoa K (2015) Hysteresis-free and highly stable perovskite solar cells produced via a chlorine-mediated interdiffusion method. J Mater Chem A 3(22):12081–12088
Green M-A, Anita H-B, Snaith H-J (2014) The emergence of perovskite solar cells. Nat Photonics 8:506–514
The authors gratefully acknowledge the financial support from the Ministry of Science and Technology of the Republic of China under Contract No. MOST 106-2221-E-027-091.
Ethics Approval and Consent to Participate
The authors declare that they have no competing interests.
Springer Nature remains neutral with regard to jurisdictional claims in published maps and institutional affiliations.
About this article
Cite this article
Chen, L., Lee, K., Wu, W. et al. Effect of Different CH3NH3PbI3 Morphologies on Photovoltaic Properties of Perovskite Solar Cells. Nanoscale Res Lett 13, 140 (2018) doi:10.1186/s11671-018-2556-8
- Solar cells
- Two-step deposition